Mat.No. 1.2080, DIN X210Cr12, AISI D3
Designation by Standards Mat. No. DIN EN AISI 1.2080 X210Cr12 - D3 Chemical Composition (in weight %) C Si Mn Cr Mo Ni V W Others 2.05 0.25 0.30 11.50 - - - - - Description D3 is an oil hardening, high carbon/chromium type tool steel with very high wear resistance. It hardens with a very slight change in size. The alloy possesses very high compressive strength and is deep hardening. Applications Cutting tools, stamping, woodworking, drawing, deep drawing and pressing tools, co...
Designation by Standards
Chemical Composition (in weight %)
D3 is an oil hardening, high carbon/chromium type tool steel with very high wear resistance. It hardens with a very slight change in size. The alloy possesses very high compressive strength and is deep hardening.
Cutting tools, stamping, woodworking, drawing, deep drawing and pressing tools, cold working rolls, measuring tools.
Physical properties (avarage values) at ambient temperature
Modulus of elasticity [103 x N/mm2]: 210
Density [g/cm3]: 7.67
Thermal conductivity [W/m.K]: 20.0
Electric resistivity [Ohm mm2/m]: 0.65
Specific heat capacity[J/g.K]: 0.46
Coefficient of Linear Thermal Expansion 10-6 oC-1
Continuous Cooling Transformation (CCT) Diagram
Time-Temperature Transformation (TTT) Diagram
Heat to 800-840oC, cool slowly. This will produce a maximum Brinell hardness of 250. To secure uniform softness.
Stress relieving to remove machining stresses should be carried out by heating to 650oC, holding for one hour at heat, followed by air cooling. This operation is performed to reduce distortion during heat treatment.
Harden from a temperature of 940-980oC followed by oil quenching or warm bath approx. 400oC. Hardness after quenching is 64-66 HRC.
For small parts up to thickness 30 mm. Harden from a temperature of 960-100oC followed by air, comompressed air quenching. Hardness after quenching is 63-65 HRC.
Tempering temperature: 150-400oC.
Tempering Temperature (oC) vs. Hardness (HRC)
Hot forming temperature: 1050-850oC.
The machinability rating of D3 is roughly 25 % that of free machining carbon steel 1018. Due to its abrasion resistant nature, machining in the hardened condition should be limited to finish grinding.
The information and data presented herein are typical or average values and are not a guarantee of maximum or minimum values. Applications specifically suggested for material described herein are made solely for the purpose of illustration to enable the reader to make his own evaluation and are not intended as warranties, either express or implied, of fitness for these or other puposes. There is no representation that the recipient of this literature will receive updated editions as the become available.